ABCD Arq Bras Cir Dig Original Article
TENSIOMETRIC ANALYSIS OF MESHES USED IN ABDOMINAL
VENTRAL WALL DEFECTS IN RATS
Estudo tensiométrico de telas utilizadas na correção de defeito na parede abdominal ventral de ratos
Carlos Alberto Lima UTRABO1,2, Nicolau Gregori CZECZKO1, Cesar Roberto BUSATO2,
Mário Rodrigues MONTEMÓR-NETTO2, Leandro LIPINSKI2, Osvaldo MALAFAIA1
From the 1Programa de Pós-Graduação em
Princípios da Cirurgia, Faculdade Evangélica
do Paraná, Curitiba, PR and 2Faculdade de
Medicina, Universidade Estadual de Ponta
Grossa (Postgraduate Program in Principles
of Surgery, Evangelic Faculty of Paraná and
Medical School, State University of Ponta
Grossa), Ponta Grossa, PR, Brazil
HEADINGS - Surgical mesh. Polypropylene.
Polyglecaprone. Tensiometry. Abdominal
ABSTRACT - Background: Among the various strategies to avoid exaggerated foreign body reaction in the
treatment of hernias is the limitation of the amount of polypropylene or the use of absorbable material. Aim:
To evaluate the healing of defects in the abdominal wall of rats, comparing microporous polypropylene,
macroporous polypropylene and polypropylene/polyglecaprone at the 30º, 60º and 120º postoperative
day. Methods: Wistar rats were submitted to defect production in the ventral abdominal wall, with integrity
of the parietal peritoneum. Prolene®, Ultrapro® and Bard Soft® meshes were used in the correction of the
defect. Nine subgroups of 10 animals were submitted to euthanasia at 30th, 60th and 120th postoperative
day. Fragments of the abdominal wall of the animals were submitted to tensiometric analysis. Results:
The tensiometry at the 30th postoperative day showed greater resistance of the tissues with Bard Soft®
(macroporous mesh) in relation to the tissues with Prolene® (microporous mesh). On the 60th postoperative
day Bard Soft® maintained the superior resistance to the tissues comparing to Prolene Mesh®. On the 120th
postoperative day the tissues repaired with Ultrapro® (macroporous mesh) proved to be more resistant than
the ones by Prolene® (microporous mesh) and Bard Soft® (macroporous mesh). Conclusion: The tissues
repaired with macroporous meshes showed greater resistance than with microporous meshes at all stages,
and at 120 days postoperative Ultrapro® performed better than the others.
RESUMO – Racional: Dentre as várias estratégias para evitar exagerada reação de corpo estranho
no tratamento das hérnias está a limitação da quantidade de polipropileno na tela ou utilização
de material absorvível. Objetivo: Avaliar a cicatrização de defeito em parede abdominal de
ratos, comparando-se as telas de polipropileno microporosa, polipropileno macroporosa e
polipropileno/poliglecaprone. Métodos: Em 90 ratos Wistar foi produzido defeito na parede
abdominal ventral, com integridade do peritônio parietal. Na correção foram utilizadas as
telas Prolene®, Ultrapro® e Bard Soft®. Nove subgrupos de 10 animais foram submetidos
à eutanásia no 30º, 60º e 120º dia do pós-operatório. Fragmentos da parede abdominal dos
animais foram submetidos à análise tensiométrica. Resultados: A tensiometria aos 30dias
mostrou maior resistência do tecido com tela Bard Soft® em relação à de Prolene®; no 60º
dia a Bard Soft® manteve a resistência superior ao Prolene®; no 120º dia a reparação com
tela macroporosa Ultrapro® mostrou-se mais resistentes que a de Prolene® e Bard Soft®.
Conclusão: Os tecidos reparados com telas macroporosas demonstraram maior resistência do
que as microporosas em todas as fases, sendo que aos 120 dias de pós-operatório a Ultrapro®
teve melhor desempenho que as demais.
Carlos Alberto Lima Utrabo
Financial source: none
Conflict of interest: none.
Received for publication:12/04/2017
Accepted for publication: 18/07/2017
DESCRITORES - Tela cirúrgica. Polipropileno.
Poliglecaprone. Tensiometria. Hérnia. Ratos.
The standard procedure for the surgical correction of the incisional hernia is performed with the use of meshes3,7,12. The most widely used material is polypropylene which causes rapid acute inflammatory response followed
by chronic foreign body reaction that persists for months and years after the surgical
procedure. Among the various strategies used to avoid exaggerated foreign body reaction
is the limitation of the amount of polypropylene or the use of absorbable material that
provides initial resistance and is quickly reabsorbed by reducing local inflammation14.
Studies focusing on the behavior of macroporous prosthetic material, including
polypropylene, have been focused on the geometry and quantity of the implanted
material. Attempts to reduce the amount of foreign body focused on the design of the
macropores and the absorbable and nonabsorbable components of the meshes. The
new designs promoted the development of the classification of the meshes as high,
medium and low weight, respectively values above 80 g/m², between 50-80 g/m² or
below 50 g/m². Some authors define as ultra light material with a density below 35 g/
m². The pore size represents an important factor for new designs, as well as the filaments
themselves and their spatial distribution6.
The most important concept in the development of hernia surgery in recent
years is the use of low weight meshes with large pores. The new generation has shown
advantages in improving postoperative comfort and in chronic postoperative pain.
The Ultrapro® represents a new member in the group of low weight with large pores.
165ABCD Arq Bras Cir Dig 2017;30(3):165-168
It consists of a monofilament with low weight and large
pores, more than 3 mm in polypropylene, with the addition
of a Monocryl® (polyglecrapone 25) absorbable component
that optimizes the implant, increasing the resistance of the
corrected wall in the first weeks after the repair. Monocryl®
is fully absorbed without increased cellularity, inflammatory
process and intense fibrotic reaction between 84-140 days.
The mesh being partially absorbable and absorbing part of its
components, reduces the amount of foreign matter without
compromising its biomechanical resistance10.
It is known that polypropylene meshes cause early and
persistent fibrosis. The reduction is directly proportional to the
reduction of its weight and the formation of the fibrosis bridges,
inversely proportional to the size of the pores11.
The present experiment aimed to study the effect of
the application of absorbable and non-absorbable meshes as
reinforcement in the closure of preperitoneal abdominal wall
lesions in rats.
The project was submitted and approved by the Animal
Use Ethics Committee (CEUA) of the State University of Ponta
Grossa, Process nº 037/2014.
A total of 90 Wistar rats (Rattus norvergicus albinus),
males, young adults, with three months weighing 280-300 g
from the Central Biotério of the State University of Ponta Grossa
were used. The animals were divided into three groups of 30
(Prolene®, Ultrapro® and Bard Soft®). All groups underwent
similar surgical procedures. In the Prolene® group, the non-
absorbable, high-density monofilament mesh with micropores
measuring approximately 0.9 mm², composed of polypropylene
with an estimated weight of 100 g/m2 (Figures 1A and 1B) was
used. In the Ultrapro® group was used the partially absorbable,
low density monofilament with an estimated weight of 28 g/m²
with macropores of 3-4 mm in size composed of a combination
of equal parts of polypropylene and polyglecaprone (Figures
1C and 1D). In the Bard Soft® group, the non-absorbable, low
density monofilament mesh with an estimated weight of 44
g/m² with macropores of approximately 6.29 mm², composed
of polypropylene (Figures 1E and 1F), was used
Each group was divided into three subgroups of 10, with
G1, G3 and G7 with Prolene® implant being evaluated respectively
at 30, 60 and 120 postoperative days; group Ultrapro® G2, G4
and G8, evaluated on the same days; group Bard Soft®, G5, G6
and G9 in an identical manner (Table 1).
TABLE 1 - Distribution of groups and subgroups
Groups Mesh Period of time Subgroups
30 days G1
60 days G3
120 days G7
30 days G2
60 days G4
120 days G8
Bard Soft Bard Soft®
30 days G5
60 days G6
120 days G9
The rats underwent preoperative fasting of 12 h and
anesthetized with atropine sulfate (0.05 mg/kg body weight)
intraperitoneally, and after 10 min the mixture of 2% xylazine
hydrochloride (10 mg/kg) and hydrochloride of ketamine 10%
(25 mg/kg). When necessary, half the dose was repeated after
20-30 min. They were submitted to postoperative analgesia
with oral acetaminophen in the dose of 40 drops for each 500
ml of water offered in the first two days.
FIGURE 1 - Meshes used in the experiment and, next to it, their
scanning electron microscopy visualization: A and B)
Prolene®; C and D) Ultrapro®; E and F) Bard Soft®
A defect of 1x2 cm was produced in the abdominal wall,
preserving the integrity of the parietal peritoneum. Correction
was performed using each of the 1.5x2.5 cm area meshes
fixed in the extraperitoneal position through four separate
stitches of Prolene® 5-0 wire securing the mesh angles to the
aponeurosis of the abdominal wall, 0.5 cm from the edge of
the lesion, and four separate stitches interspersed with the
first ones, securing the lesion at the edges of the lesion (Figure
2 - A, B and C). The skin was sutured with intradermal 5